Abstract
Voltage or electric field induced magnetization dynamics promises low power spintronics devices. For successful operation of some spintronics devices such as magnetic oscillators and magnetization switching devices a clear understanding of nonlinear magnetization dynamics is required. Here, we report a detailed experimental and micromagnetic simulation study about the effect of excitation power on voltage induced local magnetization dynamics in an ultrathin CoFeB film. Experimental results show that the resonance linewidth and frequency remains constant, whereas cone angle of the magnetization precession increases linearly with squareroot of excitation power below threshold value, known as linear excitation regime. Above threshold power, the dynamics enters into nonlinear regime where resonance linewidth monotonically increases and resonance frequency monotonically decreases with increasing excitation power. Simulation results reveal that a strong nonlinear and incoherent magnetization dynamics are observed in our experiment above the threshold power which reduces dynamic magnetic signal by suppressing large cone angle of magnetization precession. Moreover, a significant transfer of spin angular momentum from uniform FMR mode to its degenerate spin waves outside of excitation area further restrict the cone angle of precession within only few degrees in our device. Our results will be very useful to develop allvoltagecontrolled spintronics devices.
Introduction
The recent discovery of voltagecontrolled magnetic anisotropy (VCMA) has a huge potential for the development of low power spintronics devices fully operated by voltage^{1, 2}. Several physical phenomena like control of coercive field^{3} and domain wall motion^{4, 5}, magnetization switching^{1, 6,7,8,9} and coherent ferromagnetic resonance induced by voltage^{10,11,12} have already been studied by several groups. Although various kinds of material systems have been used for these studies, the multilayer systems formed by 3dferromagnetic metals and insulating MgO are found to be one of the most promising candidates among them. In particular, magnetic tunnel junctions (MTJ) formed by CoFeB/MgO/CoFeB are the basic structure of modern spintronics devices due to their large tunneling magnetoresistance (TMR) value at room temperature^{13, 14}, which can be used in nonvolatile MRAM devices.
Precessional magnetization dynamics are called in the linear regime when cone angle of magnetization precession remains only within few degrees. When the excitation power crosses threshold value, the trajectory of the magnetization precession is strongly modified and dominated by incoherent magnetization precession, known as nonlinear magnetization dynamics^{15, 16}. The nonlinear magnetization dynamics are essential for the operation of spintronics devices such as magnetic switching devices^{6, 7, 9}, magnetic oscillators^{17}. Until now, most of the voltage induced ferromagnetic resonances are reported in the linear regime^{10,11,12, 18}. In spite of many reports on the magnetic field^{16, 19, 20} or spin torque^{15} induced nonlinear magnetization dynamic, only a single report on voltage induced nonlinear dynamics of a spatially confined CoFeB film with perpendicular magnetic anisotropy (PMA) are found^{21}. Here, we study VCMA induced nonlinear magnetization dynamics in an ultrathin CoFeB film. We locally excite magnetization dynamics and systematically increase excitation power to investigate the variation of resonance frequency, linewidth, lineshape and cone angle of precession with excitation power. We also performed micromagnetic simulations to visualize the spatial maps of dynamic magnetization at different excitation power and to understand the underlying mechanism of observed dynamic behavior as a function of excitation power. We believe that our study will be very useful to understand the nonlinear magnetization dynamics in an ultrathin ferromagnetic film under local excitation scheme.
Results
Schematic of device and working principle
Figure 1 shows the schematic diagram of the device and experimental set up. The device with MTJ structure consists of 3 nm top CoFeB layer (reference layer) and 1.4 nm bottom CoFeB layer (free layer) separated by a 2 nm thick insulating MgO layer (see methods for details). The reference layer was patterned into rectangular shape (2 × 4 µm^{2}) in the middle of a much wider (50 × 100 µm^{2}) free layer (Fig. 1). Both CoFeB layers have PMA at the interface of CoFeB/MgO due to the hybridization of Fe3d and O2p orbitals^{22, 23} and the magnitude of PMA strongly depends upon the thickness of ferromagnetic layer (inversely proportional to thickness)^{24, 25}. The PMA field value of reference layer is less than the demagnetizing field. Therefore, reference layer has inplane magnetic easy axis^{24}. On the other hand, the PMA of free layer overcomes the demagnetizing field to have a net effective PMA. Therefore, free layer has outofplane magnetic easy axis. When dc or rf voltage is applied across the MTJ, the electric field at the interface of CoFeB layers modulates charge or spin density in the Fe3d orbitals^{26,27,28}, which causes a change in PMA. This change in PMA can be thought as equivalent to a magnetic field along outofplane direction which is proportional to outofplane component of saturation magnetization (M _{z})^{10}. For our measurement, rf voltage (V _{rf}) with varying frequency (f) is applied across the MTJ through the capacitor port of bias tee (Fig. 1). When f matches with the ferromagnetic resonance frequency (f _{FMR}) of the free layer under the application of bias magnetic field (H), its magnetization oscillates around effective field direction. The rectified voltage (V _{rec}) is measured through the dc port of bias tee as a function of f varying from 2 to 9 GHz (see methods for details).
Variation of PMA field with dc voltage
To evaluate the variation of PMA field (μ _{0} H _{k}) with voltage, we measured TMR of MTJ as a function of external magnetic field magnitude (μ _{0} H) from −320 mT to +320 mT along the yaxis (Fig. 1) under various dc bias voltages (V _{b}) ranging from −0.62 V to +0.62 V. Note that positive voltage means the top electrode has positive potential with respect to the bottom electrode of MTJ. The resistance and area product (RA) for our device is about 100 kΩ.µm^{2}. The TMR of a MTJ depends upon the relative angle between the magnetizations of two CoFeB layers^{29}, i.e. \({\rm{TMR}}\propto \,\sin \,{\varphi }_{F}\), where ϕ _{F} is the angle between the magnetizations of two CoFeB layers (Fig. 2(a)). Therefore the ratio of inplane component of free layer magnetization (M _{y}) and saturation magnetization (M _{s}) can be evaluated from normalized TMR curve^{30} as \({M}_{y}\propto {M}_{s}\,\cos \,{\varphi }_{F}\). In Fig. 2(b), we plot experimentally measured normalized TMR as a function of +μ _{0} H for different values of V _{b}. At μ _{0} H = 0 mT, all the curves show their maximum values which indicates that the magnetizations of both layers are aligned almost perpendicular to each other along their easy axes as schematically shown in the same figure. As μ _{0} H increases, the magnetization of free layer starts to incline along positive yaxis. Therefore, TMRs decrease monotonically with the increase of +μ _{0} H for all bias voltages until they reach to the minimum values at around +190 mT, indicating that the magnetizations of the both CoFeB layers are aligned along the +yaxis for μ _{0} H > + 190 mT. The difference in slopes among the curves originates from the modulation of μ _{0} H _{k} by V _{b} through VCMA effect^{31}. We evaluate μ _{0} H _{k} for each value of V _{b} by using the method mentioned in refs 18, 30 and 31. The effective value of μ _{0} H _{k} at V _{b} = 0 V is about 185 mT. In Fig. 2(c), we plot μ _{0}ΔH _{k}, defined by the difference between μ _{0} H _{k} at certain bias voltage and zero bias voltage, as a function of V _{b}. The magnitudes of the gradients of \({\mu }_{0}{\rm{\Delta }}{H}_{k}\) are 45 and 23 mT/V for negative and positive V _{b}, respectively. The difference between the slopes of μ _{0}ΔH _{k} for negative and positive V _{b} originates probably due to the two different interfaces (CoFeB/MgO & CoFeB/Ta) of free CoFeB layer in the MTJ^{22, 31}.
Resonance lineshape and linewidth at lower excitation power
We measured V _{rec} as a function of f for different magnitudes of +μ _{0} H. Figure 2(d) shows a typical plot of V _{rec} as a function of f measured at μ _{0} H = 100 mT and rf power (P _{rf}) = 5 µW. The rf power is low enough to excite FMR in the linear regime. The plot shows two resonance peaks. The resonance peak at 4.72 GHz with large peaktopeak height (V _{pp}) corresponds to FMR of free layer, whereas the resonance peak at 6.75 GHz with very small value of V _{pp} corresponds to FMR of reference layer. This shows that the reference layer is not efficiently excited by voltage due to near inplane orientation of magnetization. Note that very low tunneling current density (~10^{6} A.m^{−2}) can not excite reference layer by spin transfer torque (STT) or field like torque (FLT). The FMR spectrum of free CoFeB layer (Fig. 2(d)) can be fitted by linear combination of symmetric and antisymmetric Lorentzian functions given by refs 18, 32, 33:
where, V _{s} and V _{as} are the amplitudes of symmetric and antisymmetric terms, σ is the half width at half maximum (HWHM) of the spectrum and f _{FMR} is the FMR frequency. For homodynedetected signal, V _{s} originates from STT induced FMR, whereas V _{as} originates from the FMR induced by VCMA torque and/or FLT^{18, 33, 34}. Peaktopeak height (V _{pp}) of V _{rec} curves can be obtained by summing up V _{s} and V _{as}. Equation 1 fits well with the experimental resonance spectrum of free layer as shown by solid line in Fig. 2(d). According to the fitting result, V _{as} is around ten times larger than V _{s}. Therefore, the contribution of STT is negligible or much smaller than the combined effect of VCMA torque and FLT. For further confirmation, we plot peaktopeak value (V _{pp}) of V _{rec} as a function of angle (ϕ _{F}) made by free layer with film plane (see supplementary for details). The VCMA torque induced homodyne signal amplitude should be proportional to sin^{2} ϕ _{F} cos ϕ _{F} (refs 10 and 21), where V _{pp} should be maximum at ϕ _{F} ~ 55°. The maximum value of V _{pp} in our sample is obtained for ϕ _{F} ~ 59°, which implies voltage excitation of magnetization dynamics. The small deviation from theoretical value may occur due to the stray magnetic field from reference layer^{10}.
Next, we discuss about the linewidth (HWHM) of FMR spectra. The HWHM (σ) of the measured FMR spectra can be expressed as^{35}
Here, σ _{in} is the intrinsic linewidth, which originates from intrinsic Gilbert damping, σ _{ex} is the extrinsic linewidth, which originates from various extrinsic contributions and α is the intrinsic Gilbert damping constant. The intrinsic linewidth is proportional to the f _{FMR}. According to the literature^{24}, the intrinsic damping constant of 1.4 nm CoFeB is about 0.02, which gives the intrinsic resonance linewidth (σ _{in}) of about 100 MHz in absence of any extrinsic contribution. We extracted the value of σ as 425 MHz from the fitting of resonance spectrum with Eq. 1. This broad resonance linewidth in our device indicates the presence of other extrinsic contributions, which may originate from inhomogeneous distribution of PMA and/or twomagnon scattering. In our case, the device was postannealed at 300 °C in vacuum for 1 hour. Therefore, the PMA is expected to be uniform throughout the film. Twomagnon scattering which originates from the defects at the interfaces^{36, 37}, may be present only if M _{ s } is aligned at an angle (ϕ _{F}) less than 45° with respect to film plane^{37}. In our case, twomagnon scattering has negligible contribution as ϕ _{F} = 58° (>45°) (see supplementary informations). In this study, the magnetization dynamics are locally excited in the centre of a wider thin film, where spin waves are also excited outside the excitation area in addition to uniform FMR underneath the excitation area (see supplementary informations). The eigenfrequencies of the uniform FMR and spin wave modes are almost degenerated due to the small thickness of CoFeB film. This opens up a new channel for relaxation of spins correspond to uniform FMR via spin waves. Therefore, the resonance peak of uniform FMR mode is broadened. Probably, this broad peak of uniform FMR mode and other spin wave modes are not well resolved in our experiment. Therefore, we observed a single and broad resonance peak in our device instead of many isolated peaks.
Resonance spectra as a function of excitation power
We measured resonance spectra for different values of P _{rf} ranging from 5 µW to 1.41 mW at μ _{0} H = 100 mT. In static condition, the free layer magnetization is oriented at an angle of 32° with respect to the film normal at this magnetic field value. We plot V _{rec}, rescaled by a factor of 1/P _{rf}, as a function of f for different values of P _{rf} in Fig. 3(a). With the increase of P _{rf}, the resonance linewidth is broadened maintaining antisymmetric Lorentzian shape and the resonance frequency (f _{FMR}) shifts towards the lower frequency. These features may be the fingerprints of nonlinear magnetization dynamics. However, we didn’t observe hysteresis between the resonance spectra for upward and downward sweeps of f (see supplementary information) in our MTJ unlike the previous reports^{15, 20}. The reason behind this is probably thermal fluctuation of magnetizations due to Joule heating^{15, 21}.
We fitted the resonance spectra with Eq. 1 to find out the parameters V _{s}, V _{as}, f _{FMR} and σ. Figure 3(b) shows the plot of peaktopeak height (V _{pp}) of V _{rec} curves as a function of P _{rf}. The inset graph shows that the V _{pp} linearly increases with P _{rf} up to about P _{rf} = 30 μW. However, V _{pp} deviates from linear increment at higher values of P _{rf}. In Fig. 3(c), we represent variation of f _{FMR} as a function of V _{rf}, where V _{rf} = (P_{rf}Z_{0})^{1/2} is the input rf voltage and Z _{0} (=50 Ω) is the characteristic impedance of waveguide. The graph shows that f _{FMR} remains almost constant (4.72 GHz) up to V _{rf} ≈ 0.04 V, (which correspond to 32 μW of rf power) and then monotonically (linearly) decreases with the increase of V _{rf}. We also plot HWHM as a function of V _{rf} in Fig. 3(d). The HWHM remains almost constant (~425 MHz) up to V _{rf} ≈ 0.04 V. After that, HWHM increases almost linearly with the increase of V _{rf}.
Cone angle of precession
We also roughly estimated cone angle of precession in experiment from peaktopeak (V _{pp}) value of resonance spectra by using the following expression^{10, 21}:
Here, θ _{c} is the cone angle of precession, r _{TMR} = (R _{AP}−R _{P})/R _{P}, R _{P} and R _{AP} are resistances for parallel and antiparallel orientations of magnetization respectively, R is the resistance at μ _{0} H = 100 mT and Z _{0} is the characteristics impedance of waveguide. Figure 4(a) shows the plot of the θ _{c} as a function of V _{rf}. Graph shows that θ _{c} linearly increases with V _{rf} up to V _{rf} = 0.04 V, which corresponds to P _{rf} ≈ 32 µW. Above 32 µW, θ _{c} deviates from linear increment with V _{rf} and becomes almost saturated above V _{rf} ≈ 0.27 V (P _{rf} ≈ 1.41 mW), where we get the maximum value of θ _{c} of about 4.35°. All these observations suggest that P _{rf} ≈ 32 µW (V _{rf} ≈ 0.04 V) is the threshold value of rf power above which the dynamics enters into nonlinear regime.
Micromagnetic simulations
To understand the underlying mechanism of the observed dynamic behaviours as a function of P _{rf}, we performed micromagnetic simulations^{38} based on LandauLifshitzGilbert (LLG) equation (see methods). In the simulations, magnetization dynamics were excited by applying sinusoidal rf magnetic field (h _{rf} sin 2πft) along zaxis with frequency f only in the central 2 × 4 µm^{2} area of CoFeB layer highlighted by green colour in Fig. 5(a). The magnitudes (h _{rf}) of rf magnetic field were taken to be equivalent to the PMA field modulated by applied V _{rf} as calculated from experimental result presented in Fig. 2(c) and Eq. 4 given below^{21}.
Here, \(\frac{\partial {H}_{k}}{\partial {V}_{b}}=34.2\mathrm{mT}/V\) is the average gradient of μ _{0}ΔH _{k} for positive and negative V _{b}, Γ = (R − Z _{0})/(R + Z _{0}) is the reflection coefficient of V _{rf} from the MTJ. The experimentally measured rectified voltage (V _{rec}) can be expressed as the timeaveraged value of the product of oscillating TMR due to precession of magnetization and rf tunnel current as given below^{18, 33}
where, R is the resistance, p is a spin polarization (we used 0.5), and ϕ _{F}(t) is timedependent relative angle between the magnetizations in the free and reference CoFeB layers. As the orientation of reference layer magnetization is nearly inplane of the film, we simply adopt the angle (ϕ _{F}) made by free layer with the film plane as equals to the angle made by free layer with the reference layer. R(t) = R/(1 + p ^{2} cos θ _{F}(t)) represents the timedependent resistance due to oscillation of ϕ _{F} and I _{rf}(t) = V _{rf}sin(2πft)/R represents the timedependent tunnel current. Therefore, experimentally measured V _{rec} can be reproduced by micromagnetic simulations by using the time variation of ϕ _{F} when applying V _{rf}. Note that ϕ _{F} is the angle made by average magnetization of the green area (Fig. 5(a)) with the film plane. We used α = 0.02 in the simulation.
Figure 5(b) shows the plot of simulated rectified voltage (V _{rec}), rescaled by a factor of 1/P _{rf}, as a function of excitation frequency (f) for different values of P _{rf}. The simulated resonance spectra also look like antisymmetric Lorentzian in the linear or lower power (up to 36 μW) regime. With the increase of P _{rf} the resonance spectra are broadened gradually like experimental results. The spectra also show decrease of f _{FMR} and peaktopeak height of V _{rec}/P _{rf} curves with P _{rf} similar to the experimental results. To get into the more details of the underlying mechanism, we show snapshots of the spatial distribution of dynamic magnetization for different values of P _{rf} in Fig. 5(c). The snapshots show that the dynamics is uniform and coherent up to 36 μW of rf power. Above 36 μW, the dynamics starts to become nonuniform and incoherent. The degree of incoherence gradually increases with further increase of P _{rf}. The snapshots clearly show a smooth transition from coherent or linear magnetization dynamics to incoherent or nonlinear magnetization dynamics with a threshold power of about 36 μW. Therefore the dynamic dephasing due to the incoherent nonlinear dynamics reduces peaktopeak height (V _{pp}) of rectified voltage (V _{rec}). Hence we observe a deviation of V _{pp} from linear increment with P _{rf} and deviation of θ _{c} from linear increment with V _{rf} above threshold value of P _{rf} in experiment as well as in simulation results. Note that this dynamic dephasing also broadens resonance linewidth.
In Fig. 4(b) we also plot simulated value of θ _{c} as a function of V _{rf}. The graph shows that θ _{c} linearly increases with V _{rf} up to V _{rf} = 0.04 V (P _{rf} ≈ 32 µW). Above the threshold power of 32 µW, θ _{c} deviates from linear increment with V _{rf} and becomes almost saturated above V _{rf} ≈ 0.25 V (P _{rf} ≈ 1.25 mW), where we get the maximum value of θ _{c} of about 12°. It shows that simulation result qualitatively reproduces the experimental result about the variation of θ _{c} with V _{rf} (Fig. 4(a)). However, simulation result shows much larger cone angle of precession as opposed to the experiment. This can be explained in the following way. We observed broad resonance linewidth in experiment due to the spin wave generation outside the excitation area. In this way spin angular momentum corresponds to uniform FMR mode is transferred to its degenerate spin waves. Therefore in our experiment, the cone angle of precession corresponds to uniform FMR can not go beyond 4.35° even at very high excitation power. For exact reproduction of experimental result all the external parameters like extrinsic contributions of damping, temperature, stray field from reference layer and other boundary conditions have to be taken into account, which is not possible in OOMMF simulation. Therefore, broad resonance linewidth due to extrinsic contributions like spin wave generation can not be reproduced in micromagnetic simulations. That is why the cone angle of precession in simulation can reach up to 12° unlike experiment.
We further plot simulated values of f _{FMR} as a function of V _{rf} in Fig. 3(c). The simulated results also show that f _{FMR} remains almost constant up to about V _{rf} = 0.04 V (threshold power). Above threshold power, f _{FMR} decreases almost linearly with V _{rf} like the experimental result due to the nonlinear dynamics. However, we observed a steeper variation of f _{FMR} with V _{rf} in the simulation than that of the experiment. In the linear regime, the precessional axis of the magnetization makes an angle of 32° with respect to outofplane direction which is essentially the direction of the effective magnetic field (H _{eff}) determined by bias magnetic field, PMA field and demagnetizing field. With the increase of P _{rf}, the cone angle of precession increases which in fact decreases M _{z} (ref. 15). Therefore, H _{eff} and hence f _{FMR} decreases with the increase of P _{rf}. In our simulation, the steeper decrease of f _{FMR} with V _{rf} was observed mainly due to the larger cone angle of precession as opposed to the experiment. A complete quantitative reproduction of experimental results is not possible as the effect of Joule heating and extrinsic contributions to the resonance linewidth can not be taken into account. These Joule heating may also change the PMA of CoFeB film. Therefore the simulation result may differ from experimental results. Nevertheless, the micromagnetic simulations qualitatively reproduce all the important features of dynamics behaviour observed in the experiment.
Discussions
A complete knowledge about the voltage induced nonlinear magnetization dynamics is essential for the application in future spintronics devices. However, the behaviour of nonlinear magnetization dynamics is quiet different than that of the linear dynamics. The magnetization dynamics in the nonlinear regime are governed by second order Suhl process^{16, 39} or four magnon scattering. In this process two k = 0 magnons are annihilated to create two k ≠ 0 (+k and −k) magnons^{19, 40}. In other words a spontaneous transfer of angular momentum from coherent uniform precession of magnetizations to incoherent nonuniform precession of magnetizations occurs. This agrees with the observed behaviour in micromagnetic simulations. The dynamic dephasing among these incoherent k ≠ 0 magnons decreases the amplitude (V _{pp}) or cone angle of precession (θ _{c}) of dynamic magnetization than that of the expected values. The relaxation of magnetization dynamics in the nonlinear regime is also governed by intrinsic four magnon scattering^{40}. The spin relaxation rate increases with the increase of four magnon scattering^{39}. Again, the linewidth of the resonance spectra is linearly proportional to the relaxation rate. As the four magnon scattering process increases with the increase of P _{rf}, we observed a monotonic increment of HWHM as a function of V _{rf} or P _{rf}.
In conclusion, we have shown a systematic transition from linear magnetization dynamics to nonlinear magnetization dynamics for local excitation of magnetization by experiment and micromagnetic simulation study. Simulations results demonstrate that the coherent and linear magnetization dynamics becomes incoherent and nonlinear above a certain threshold value of rf power. This incoherent nonlinear dynamics significantly reduces dynamic signal i.e. cone angle of magnetization precession and increases resonance linewidth. Voltage induced local magnetization dynamics is essential for exciting spin waves in future spintronics devices. We show that locally excited uniform magnetization dynamics also excites spin waves, almost degenerate to uniform FMR mode, outside the excitation area in ultrathin magnetic films. The resonance linewidth correspond to uniform FMR mode is enhanced due to the channelling of angular momentum from uniform FMR inside excitation area to spin wave mode outside the excitation area. We have further shown that this broad resonance linewidth does not allow cone angle of magnetization precession to exceed only above few degrees in our device. We think our study will be very useful for the development of allvoltagecontrolled spin waves based logic devices.
Methods
Sample fabrication
The devices were fabricated by a multistep fabrication method. At first, filmstacking structure used in this study were prepared on a thermally oxidized Si(001) substrate by rf sputtering at room temperature at a base pressure of 10^{−9} Torr. The structure consists of the following layers (nominal thicknesses in nanometres are stated in parentheses): Si/Ta(5)/Ru(20)/Ta(5)/Co_{20}Fe_{60}B_{20}(1.4)/MgO(2)/Co_{20}Fe_{60}B_{20}(3)/Ta(5)/Ru(5). In second step, the free layers with dimension 50 × 100 μm^{2} were defined by maskless photolithography followed by Ar^{+} ion milling down to Sisubstrate. In the third step, reference layers with dimension 2 × 4 μm^{2} were defined in the middle of free layers (Fig. 1(a)) by maskless photolithography followed by Ar^{+} ion milling down to MgO layer and subsequent deposition of 40 nm thick Al_{2}O_{3}. The dimension of reference layer defines the dimension of MTJ. In the fourth step, 100 nm thick Al_{2}O_{3} was deposited everywhere except on top of the reference layer (for top electrode) and in the vicinity of the edge of free layer (for bottom electrode). Finally, the contacts were designed by photolithography followed by deposition of Ti(5)/Au(100) by electron beam evaporation. Fabricated devices were postannealed at 300 °C in vacuum under a perpendicular magnetic field of 600 mT for one hour. High temperature annealing over 300 °C decreased µ_{0} H _{k} due to intermixing of the interface between CoFeB and Ta^{41}. For a good thermal stability of the surface magnetic anisotropy, one can use W buffer layer instead of Ta^{42}.
Experimental Measurement
The ferromagnetic resonance in CoFeB layers were excited by applying rf voltage across the MTJ. The rf voltage (V _{rf}) produces rf electric field (E _{rf}) at the interfaces of the CoFeB/MgO junction. The E _{rf} modulates interfacial PMA of CoFeB layer. When frequency of V _{rf} matches the FMR frequency (f _{FMR}) of free layer, magnetization dynamics is excited. Magnetization dynamics produces an oscillatory TMR (depends upon the relative angle between the magnetizations of two layers) at the same frequency than that of the V _{rf}. The mixing of oscillatory TMR and small rf tunnel current generates finite dc voltage (called as rectified voltage), which is measured by a multimeter connected to the dc port of the bias tee. To remove the background not coming from FMR, we measured reference spectra at μ _{0} H = 300 mT correspond to each rf power (P _{rf}) and subtracted from spectrum corresponds to each bias magnetic field and P _{rf}. At μ _{0} H = 300 mT, the magnetizations of free layer and reference layer are expected to be parallel to each other. Therefore precession of free layer magnetization does not produce any timedependent TMR.
Micromagnetic Simulations
The micromagnetic simulations were performed by using Object Oriented Micromagnetic Framework (OOMMF) software based on LandauLifshitzGilbert equation of motion^{38} given by:
The STT term is neglected because of its small contribution in our MTJ. In this equation, M is saturation magnetization, γ is the gyromagnetic ratio, α is the Gilbert damping constant and H _{ eff } is the effective magnetic field composed of bias magnetic field, PMA field and demagnetizing field. For the simulations, a model sample with dimension 10 µm (x) × 10 µm (y) × 1.4 nm (z) was considered (Fig. 5(a)). The mess size was taken as 20 nm × 20 nm × 1.4 nm. We adopted the anisotropy energy density of 1.012 × 10^{5 }J/m^{3} in outofplane direction, saturation magnetization µ _{0} M _{s} of 1.5 T, gyromagnetic ratio of 28 GHz.T^{−1} and exchange stiffness constant of 20 pJ.m^{−1}. The exchange stiffness constant was found from ref. 43, whereas other parameters were extracted from experimental results (see supplementary information). At first, the ground state of magnetization was prepared by applying a bias magnetic field along ydirection. The magnetization dynamics was then excited by applying a sinusoidal rf magnetic field (h _{z} = h _{rf} sin 2πft) (Eq. 4) with frequency f. As V _{rf} modulates PMA of free CoFeB layer only in the area underneath the reference CoFeB layer, h _{z} was applied only in the central 2 × 4 µm^{2} area of CoFeB layer marked by green colour in Fig. 5(a). The magnitudes of h _{z} i.e. h _{rf} were chosen equivalent to the PMA field modulated by applied V _{rf} as calculated from experimental result shown in Fig. 2(b) and Eq. 4. The time varying average magnetization components were also extracted from the green area to mimic the experimental condition.
References
 1.
Maruyama, T. et al. Large voltageinduced magnetic anisotropy change in a few atomic layers of iron. Nat. Nanotechnol. 4, 158–161, doi:10.1038/nnano.2008.406 (2009).
 2.
Suzuki, Y., Kubota, H., Tulapurkar, A. & Nozaki, T. Spin control by application of electric current and voltage in FeCo–MgO junctions. Phil. Trans. R. Soc. A 369, 3658–3678, doi:10.1098/rsta.2011.0190 (2011).
 3.
Seki, T., Kohda, M., Nitta, J. & Takanashi, K. Coercivity change in an FePt thin layer in a Hall device by voltage application. Appl. Phys. Lett. 98, 212505, doi:10.1063/1.3595318 (2011).
 4.
Schellekens, A. J., van den Brink, A., Franken, J. H., Swagten, H. J. M. & Koopmans, B. Electricfield control of domain wall motion in perpendicularly magnetized materials. Nat. Commun. 3, 847, doi:10.1038/ncomms1848 (2012).
 5.
Bauer, U., Emori, S. & Beach, G. S. D. Voltagegated modulation of domain wall creep dynamics in an ultrathin metallic ferromagnet. Appl. Phys. Lett. 101, 172403, doi:10.1063/1.4764071 (2012).
 6.
Kanai, S. et al. Electric fieldinduced magnetization reversal in a perpendicularanisotropy CoFeBMgO magnetic tunnel junction. Appl. Phys. Lett. 101, 122403, doi:10.1063/1.4753816 (2012).
 7.
Wang, W., Li, M., Hageman, S. & Chien, C. L. Electricfieldassisted switching in magnetic tunnel junctions. Nat. Mater. 11, 64–68, doi:10.1038/nmat3171 (2012).
 8.
Yoichi, S. et al. Voltageassisted magnetization switching in ultrathin Fe_{80}Co_{20} alloy layers. Appl. Phys. Express 2, 063001, doi:10.1143/APEX.2.063001 (2009).
 9.
Shiota, Y. et al. Induction of coherent magnetization switching in a few atomic layers of FeCo using voltage pulses. Nat. Mater. 11, 39–43, doi:10.1038/nmat3172 (2012).
 10.
Nozaki, T. et al. Electricfieldinduced ferromagnetic resonance excitation in an ultrathin ferromagnetic metal layer. Nat. Phys. 8, 491–496, doi:10.1038/nphys2298 (2012).
 11.
Kanai, S., Gajek, M., Worledge, D. C., Matsukura, F. & Ohno, H. Electric fieldinduced ferromagnetic resonance in a CoFeB/MgO magnetic tunnel junction under dc bias voltages. Appl. Phys. Lett. 105, 242409, doi:10.1063/1.4904956 (2014).
 12.
Miura, K. et al. Voltageinduced magnetization dynamics in CoFeB/MgO/CoFeB magnetic tunnel junctions. Sci. Rep. 7, 42511, doi:10.1038/srep42511 (2017).
 13.
Hayakawa, J., Ikeda, S., Lee, Y. M., Matsukura, F. & Ohno, H. Effect of high annealing temperature on giant tunnel magnetoresistance ratio of CoFeB/MgO/CoFeB magnetic tunnel junctions. Appl. Phys. Lett. 89, 232510, doi:10.1063/1.2402904 (2006).
 14.
Ikeda, S. et al. Tunnel magnetoresistance of 604% at 300K by suppression of Ta diffusion in CoFeB∕MgO∕CoFeB pseudospinvalves annealed at high temperature. Appl. Phys. Lett. 93, 082508, doi:10.1063/1.2976435 (2008).
 15.
Chen, W., de Loubens, G., Beaujour, J.M. L., Sun, J. Z. & Kent, A. D. Spintorque driven ferromagnetic resonance in a nonlinear regime. Appl. Phys. Lett. 95, 172513, doi:10.1063/1.3254242 (2009).
 16.
Bi, C. et al. Electrical detection of nonlinear ferromagnetic resonance in single elliptical permalloy thin film using a magnetic tunnel junction. Appl. Phys. Lett. 99, 232506, doi:10.1063/1.3670302 (2011).
 17.
Kiselev, S. I. et al. Microwave oscillations of a nanomagnet driven by a spinpolarized current. Nature 425, 380–383, doi:10.1038/nature01967 (2003).
 18.
Zhu, J. et al. Voltageinduced ferromagnetic resonance in magnetic tunnel junctions. Phys. Rev. Lett. 108, 197203, doi:10.1103/PhysRevLett.108.197203 (2012).
 19.
Bauer, H. G., Majchrak, P., Kachel, T., Back, C. H. & Woltersdorf, G. Nonlinear spinwave excitations at low magnetic bias fields. Nat. Commun. 6, 8274, doi:10.1038/ncomms9274 (2015).
 20.
Gui, Y. S., Wirthmann, A., Mecking, N. & Hu, C. M. Direct measurement of nonlinear ferromagnetic damping via the intrinsic foldover effect. Phys. Rev. B 80, 060402, doi:10.1103/PhysRevB.80.060402 (2009).
 21.
Hirayama, E. et al. Electricfield induced nonlinear ferromagnetic resonance in a CoFeB/MgO magnetic tunnel junction. Appl. Phys. Lett. 107, 132404, doi:10.1063/1.4932092 (2015).
 22.
Shimabukuro, R., Nakamura, K., Akiyama, T. & Ito, T. Electric field effects on magnetocrystalline anisotropy in ferromagnetic Fe monolayers. Phys. E 42, 1014–1017, doi:10.1016/j.physe.2009.11.110 (2010).
 23.
Yang, H. X. et al. Firstprinciples investigation of the very large perpendicular magnetic anisotropy at Fe/MgO and Co/MgO interfaces. Phys. Rev. B 84, 054401, doi:10.1103/PhysRevB.84.054401 (2011).
 24.
Ikeda, S. et al. A perpendicularanisotropy CoFeB–MgO magnetic tunnel junction. Nat. Mater. 9, 721–724, doi:10.1038/nmat2804 (2010).
 25.
Iihama, S. et al. Gilbert damping constants of Ta/CoFeB/MgO(Ta) thin films measured by optical detection of precessional magnetization dynamics. Phys. Rev. B 89, 174416, doi:10.1103/PhysRevB.89.174416 (2014).
 26.
Duan, C. et al. Surface magnetoelectric effect in ferromagnetic metal films. Phys. Rev. Lett. 101, 137201, doi:10.1103/PhysRevLett.101.137201 (2008).
 27.
Nakamura, K. et al. Giant modification of the magnetocrystalline anisotropy in transitionmetal monolayers by an external electric field. Phys. Rev. Lett. 102, 187201, doi:10.1103/PhysRevLett.102.187201 (2009).
 28.
Tsujikawa, M. & Oda, T. Finite electric field effects in the large perpendicular magnetic anisotropy surface Pt/Fe/Pt(001): a firstprinciples study. Phys. Rev. Lett. 102, 247203, doi:10.1103/PhysRevLett.102.247203 (2009).
 29.
Slonczewski, J. C. Conductance and exchange coupling of two ferromagnets separated by a tunneling barrier. Phys. Rev. B 39, 6995–7002, doi:10.1103/PhysRevB.39.6995 (1989).
 30.
Yoichi, S. et al. Quantitative evaluation of voltageinduced magnetic anisotropy change by magnetoresistance measurement. Appl. Phys. Express 4, 043005, doi:10.1143/APEX.4.043005 (2011).
 31.
Takayuki, N. et al. Voltageinduced magnetic anisotropy changes in an ultrathin FeB layer sandwiched between two MgO layers. Appl. Phys. Express 6, 073005, doi:10.7567/APEX.6.073005 (2013).
 32.
Kotaro, M. et al. Size dependence of magnetic properties of nanoscale CoFeB–MgO magnetic tunnel junctions with perpendicular magnetic easy axis observed by ferromagnetic resonance. Appl. Phys. Express 6, 063002, doi:10.7567/APEX.6.063002 (2013).
 33.
Sankey, J. C. et al. Measurement of the spintransfertorque vector in magnetic tunnel junctions. Nat. Phys. 4, 67–71, doi:10.1038/nphys783 (2008).
 34.
Wang, C. et al. Bias and angular dependence of spintransfer torque in magnetic tunnel junctions. Phys. Rev. B 79, 224416, doi:10.1103/PhysRevB.79.224416 (2009).
 35.
Okada, A. et al. Electricfield effects on magnetic anisotropy and damping constant in Ta/CoFeB/MgO investigated by ferromagnetic resonance. Appl. Phys. Lett. 105, 052415, doi:10.1063/1.4892824 (2014).
 36.
Beaujour, J. M., Ravelosona, D., Tudosa, I., Fullerton, E. E. & Kent, A. D. Ferromagnetic resonance linewidth in ultrathin films with perpendicular magnetic anisotropy. Phys. Rev. B 80, 180415, doi:10.1103/PhysRevB.80.180415 (2009).
 37.
Lindner, J. et al. Twomagnon damping in thin films in case of canted magnetization: theory versus experiment. Phys. Rev. B 80, 224421, doi:10.1103/PhysRevB.80.224421 (2009).
 38.
Donahue, M. J. & Porter, D. G. OOMMF User’s Guide, Version 1.0, Interagency Report NISTIR 6376, National Institute of Standards and Technology, Gaithersburg, MD (Sept 1999), http://math.nist.gov/oommf/.
 39.
Suhl, H. The theory of ferromagnetic resonance at high signal powers. J. Phys. Chem. Solids 1, 209–227, doi:10.1016/00223697(57)900100 (1957).
 40.
Dobin, A. Y. & Victora, R. H. Intrinsic nonlinear ferromagnetic relaxation in thin metallic films. Phys. Rev. Lett. 90, 167203, doi:10.1103/PhysRevLett.90.167203 (2003).
 41.
Yamanouchi, M. et al. Dependence of magnetic anisotropy on MgO thickness and buffer layer in Co_{20}Fe_{60}B_{20}MgO structure. J. Appl. Phys. 109, 07C712, doi:10.1063/1.3554204 (2011).
 42.
Skowroński, W. et al. Underlayer material influence on electricfield controlled perpendicular magnetic anisotropy in CoFeB/MgO magnetic tunnel junctions. Phys. Rev. B 91, 184410, doi:10.1103/PhysRevB.91.184410 (2015).
 43.
Ulrichs, H., Lenk, B. & Münzenberg, M. Magnonic spinwave modes in CoFeB antidot lattices. Appl. Phys. Lett. 97, 092506, doi:10.1063/1.3483136 (2010).
Acknowledgements
We would like to thank Dr. Olivier Rousseau and Dr. Susumu Ogawa for fruitful discussions.
Author information
Affiliations
Contributions
Y.O. and H.T. supervised the study. B.R. and K.M. fabricated devices. B.R. performed measurements and numerical simulations. B.R. analyzed data and wrote the manuscript with the help of Y.F. All the authors discussed the results and commented to improve the quality of manuscript.
Corresponding author
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Rana, B., Fukuma, Y., Miura, K. et al. Effect of excitation power on voltage induced local magnetization dynamics in an ultrathin CoFeB film. Sci Rep 7, 2318 (2017). https://doi.org/10.1038/s41598017024273
Received:
Accepted:
Published:
Further reading

Dynamic electromagnonic crystal based on artificial multiferroic heterostructure
Communications Physics (2019)

Towards magnonic devices based on voltagecontrolled magnetic anisotropy
Communications Physics (2019)

Experimental Demonstration of a Spin Logic Device with Deterministic and Stochastic Mode of Operation
Scientific Reports (2018)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.